Chapter 1: Introduction
The first portion of this chapter is a brief background and statement of the
problem being examined in the current work, namely the characterization of the
mechanical behavior of mineralized tissues at fundamental, ultrastructural, length-scales.
The motivation for examining the ultrastructure of these materials will be introduced and
the gaps in existing knowledge will be presented. The second portion of this chapter is
an introduction to the materials studied in the remainder of the work, beginning with
engineering materials. Structures of the mineralized biological tissues in bones and teeth
are presented along with a brief introduction to biomimetic materials for mineralized
tissue replacement. The chapter concludes with a road map for the organization and
content of the remainder of this work.
1.1 Statement of Problem
Mineralized tissues have important structural functions in the body. Teeth are
degraded by carious disease, leading to their necessary repair or removal. The bony
skeleton can become structurally unsound, globally as in osteoporosis, or locally when
large pieces of bone are removed from the body due to malignancies or trauma.
Because these materials have important structural functions, there is obvious
motivation for studying their mechanical functioning under normal deformations as well
as conditions that induce failure. An understanding of both normal and abnormal
mechanical circumstances in vivo can assist in both the prevention of failure and in the
development of remedies post-failure. This approach to mineralized tissue is inherently
physics- or engineering-based, focused on the structural and mechanical functioning of
the connective tissue matrix as opposed to approaches that are inherently cell biological.
Many studies have examined the behavior of mineralized tissues under a variety
of mechanical loading conditions and at length-scales ranging from the macroscopic to
the microscopic. Much recent attention has been on the examination of bones and teeth
at ever-smaller length-scales, below the threshold for traditional mechanical testing and
optical examination in white light, and incorporating techniques such as electron
microscopy and atomic force microscopy for visualizing the ultrastructure and
nanoindentation testing for probing mechanical behavior.
Nanoindentation is a mechanical technique for examining materials at nanometer
to micrometer length-scales. A small indenter tip is brought down onto the surface of the
sample, and pressed into the sample surface while the load and deformation are being
continuously measured. From the load and deformation measurements, material
properties (e.g. the elastic modulus) can be calculated for the local region of the sample
contacted by the tip. This technique has great promise for the examination of
inhomogeneous materials, including biological composite materials, since properties can
be mapped out from point to point in one or two dimensions, allowing for the
examination of biological effects at length scales comparable to the cells associated with
these biological effects.
A large number of studies have been performed, primarily in the last decade,
using nanoindentation to examine local mechanical responses of mineralized tissues in
bones and teeth. Studies have examined both the baseline structure-properties
relationships for healthy tissues as well as the effects of disease state on nanomechanical
response. It was found that in osteoporosis, although the total volume of bone drops
drastically with worsening disease state, nanoindentation modulus measurements
revealed no change in the local elastic modulus of the remaining tissue [Guo and
Goldstein, 2000]. In contrast, in dental caries, substantial decreases in both dentin and
enamel elastic modulus values have been noted, in conjunction with decreases in
mineralization [Bembey et al, 2005; Angker et al, 2004].
Some studies using nanoindentation have noted substantial and surprisingly large
variability in response and obtained properties. Cuy et al  examined the variation
in elastic modulus in the enamel of a single tooth cross-section and saw values that varied
smoothly across the tooth, ranging from less than 70 GPa to greater than 115 GPa. The
modulus variations appeared to related to patterns of loading during mastication
(chewing). Zysset et al  examined variations in bone modulus at different sites in
the body and found large variations depending on tissue type and subject. The range of
observed bone modulus values was from 7 to 25 GPa. Clearly at the scale of
nanoindentation testing, nanometers to micrometers, mineralized tissues have extremely
variable local responses. These variations have clinical implications as well. In
comparing finite element models for homogeneous bone versus locally-varying bone
with the same average elastic modulus, a substantial increase in local bone failure
probabilities was seen with increasing variability of local modulus [Jaasma et al, 2000].
No comprehensive analysis of the structural causes of local mechanical variability, as
seen in indentation testing, has been performed to date.
Although nanoindentation has been widely used to examine mechanical responses
of mineralized tissues, there are some additional limitations in its current applicability
that have not been adequately addressed by the existing literature. A basic technique to
obtain elastic modulus from raw indentation data (the Oliver-Pharr method [Oliver and
Pharr, 1992]) is built into commercially-available software packages, but was designed
for stiff, homogeneous engineering materials and not biological tissues. Potential
problems associated with the application of this technique to more compliant materials
are associated with both the fundamental physics of the deformation process as well as
operational details such as calibration techniques best suited for compliant samples.
Another outstanding issue is the influence of time-dependent deformation, characteristic
of hydrated biological tissues, in the indentation response.
Potentially contributing to the observed variability in indentation responses, there
is an intrinsic uncertainty associated with the interpretation of indentation data obtained
at length-scales comparable to the nanocomposite structure of mineralized biological
tissues. It has been demonstrated that in models of indentation loading of a composite
engineering material, contact hardness results vary dramatically from what would be
inferred from a composite homogenization scheme (in which the body is assigned
uniform elastic properties calculated from the composite phase contributions) [Shen and
Guo, 2001]. Since the indentation loading is localized and inhomogeneous, the
individual local features in the composite structure are important. It is also well-known
that at the most fundamental (sub-nm to nm) length-scales, mineralized tissues are
composites composed of water, an organic protein phase, and an inorganic mineral phase.
Even with the technology developed for examination of structure at these fundamental
scales, there are a number of outstanding questions regarding the organization of these
components and in turn how this organization leads to the observed structural and
mechanical functions. Mineralized tissues have been examined at the macro-scale within
the framework of engineering composite materials, and it has been shown that
composition (mineral volume fraction) was insufficient to predict the elastic modulus of
bonelarge modulus changes are seen at nearly constant mineral volume fraction [Katz,
1971]. No study since has really improved on Katz's early work or made sense of bone
(ultra)structure-properties relationships within a composite materials framework.
Given the fact that there is poor understanding of the factors contributing to the
elastic response of mineralized tissues at the macroscale, it is perhaps not surprising that
little has been said on the difficulties of understanding nanoindentation responses of these
materials at sub-microstructural scales. There are two practical implications of this
current knowledge gap: (1) it is difficult to design biologically and clinically useful
experiments when the tool (nanoindentation) being used is poorly understood; (2) it is
difficult to design clinically-useful biomimetic materials, when one is attempting to
mimic a structure that is poorly understood.
The current work will use a combined modeling and experimental approach to
examine the indentation responses of mineralized tissues as well as more fundamental
aspects of their mechanical behavior at small scales. Particular emphasis will be placed
on the factors that contribute to point-to-point variability in indentation mechanical
The next section of this chapter will briefly describe the composition and structure
of the materials examined throughout the course of this work. Following this
introductory material will be a road map describing the organization and layout of the
remainder of this work.
1.2 Materials Background
1.2.1 Engineering Materials and Mechanical Behavior